# Elastic Plastic Materials

date post

21-Feb-2015Category

## Documents

view

206download

2

Embed Size (px)

### Transcript of Elastic Plastic Materials

NPL Manual Manual for the Calculation of Elastic-Plastic Materials Models Parameters

This Electronic Guide was produced as part of the Measurements for Materials System Programme on Design for Fatigue and Creep in Joined Systems

Introduction Testing Calculation of Parameters Typical Predictions Failure Criteria

Full contents page is available

Crown copyright 2007 Reproduced with the permission of the Controller of HMSO and Queen's Printer for Scotland

ContentsIntroduction Overview of elastic-plastic models Von Mises parameters Von Mises information Typical von Mises parameters Drucker-Prager models Linear Drucker-Prager parameter calculation Associated and non-associated flow Exponent Drucker-Prager parameter calculation Data analysis Equivalent data points Effect of equivalent data point selection on parameters Typical linear Drucker-Prager parameters Typical exponent Drucker-Prager parameters Cavitation model parameters Cavitation model information Typical cavitation model parameters Calculation of parameters Typical Predictions Scarf joint Lap joint Tpeel joint Butt joint Failure CriteriaHOME

Tensile Data input Tensile Testing Typical tensile data Tensile data for elastic-plastic models Elastic and plastic behaviour Hardening curves Calculation of parameters Shear Data input Shear Testing Typical shear data Shear data parameters Calculation of shear parameters Compression Data input Compression Testing Typical compression data Compression data calculations

INTRODUCTIONFinite element analysis is a computational tool that can be used for calculating forces, deformations, stresses and strains throughout a bonded structure. These predictions can be made at any point in the structure including within the adhesive layer. Furthermore, the element mesh can accurately describe the geometry of the bond line so the influence of geometrical features, such as the shape of fillets and boundaries with adherends, on joint performance can be accounted for in the analysis. This is particularly important in the design of adhesive joints because these features are usually associated with regions of stress and strain concentration likely to initiate joint failure. Since adhesives are generally tough materials, they can sustain large strains before failure and, under these conditions, relationships between stress and strain are highly non-linear. The origin of non-linearity in a stress-strain curve for a polymeric adhesive can be explained in terms of enhanced creep brought about by an increase in molecular mobility caused by the application of stress. At moderate stresses this non-linear deformation is recoverable. At higher stresses, the molecular mobility is high enough for yielding to occur by plastic flow, which is not recoverable. Elastic-plastic materials are employed to describe deformation under large strain. There are several models available for modelling the adhesive based on different criteria for plastic deformation. Predictions of joint performance at large strains close to joint failure depend on the model used. For the prediction of failure, stress and strain distributions in the adhesive need to be accurately calculated and a failure criterion for the adhesive needs to be established. In its current form, this manual demonstrates the calculation of parameters for use with four different elastic-plastic material models. These four elastic plastic models are: von Mises, linear Drucker-Prager, exponent Drucker-Prager and Cavitation model. Material Models Von Mises Linear Drucker-Prager Exponent Drucker-Prager Cavitation model Data requirements tensile only tensile data and shear data at the same strain rate tensile data and shear data at the same strain rate tensile data, shear data and compressive data at the same strain rate

Click here for an overview of the models

BACK

HOME

NEXT

Material models overview

Von Mises criterion is the most simple yield criterion. It interprets yielding as a purely shear deformation process which occurs when the effective shear stress reaches a critical value. Simple equations relate the tensile yield stress, shear yield stress and compressive yield stress to a material property. Tests on adhesives under additional stress states reveal that in many cases yielding is sensitive to the hydrostatic component of stress in addition to the shear component. Therefore the von Mises criterion is not realistic for many adhesives. The linear Drucker-Prager model is a simple modification of the von Mises criterion that includes some hydrostatic stress sensitivity. A parameter () is introduced which characterises the sensitivity of yielding to hydrostatic stress. Two different stress states e.g. tension and shear are required to determine this parameter. The linear Drucker-Prager model is not capable of accurately describing the non-linear behaviour of an important class of tough adhesives - the rubber toughened materials. The exponent Drucker-Prager is a more complex elastic-plastic model, which is better able to describe behaviour under stress states in which there is a high component of hydrostatic tension. Two different stress states e.g. tension and shear are required to determine the exponent Drucker-Prager hydrostatic stress sensitivity parameter. In rubber-toughened epoxy, nucleation of cavities occurs in the rubber phase. The Cavitation model includes the influence of void nucleation on ductility through adaptation of the linear Drucker-Prager model. This model has been developed at NPL and is currently being used to evaluate the accuracy of predictions of deformation in various joint geometries.

BACK

HOME

TENSILE DATA INPUT

Tensile data are required for all four elastic-plastic materials models considered here. The data obtained from tensile test measurements of bulk adhesive are nominal (or engineering) values, where stresses and strains have been calculated using the initial specimen dimensions. Measurements of the following data are required:

Nominal Stress (MPa) Nominal Axial Strain Nominal Transverse Strain

For more information on tensile testing please click here

Typical data for a rubber-toughened epoxy

BACK

HOME

NEXT

Tensile TestingTensile tests [1] for the determination of Young's modulus (E') and Poisson's ratio () are carried out on standard specimens [2, 3] under constant deformation rate in a tensile test machine at relatively low strain rates e.g. 10 mm/min. For best accuracy, contacting extensometers should be used for the measurement of axial and transverse strain, T and t. Two extensometers mounted on opposite faces of the specimen should preferably be used for the axial strain measurement to eliminate small non-uniformity in the strain through the thickness of the specimen caused by bending. The transverse strain measurement should be made close to the axial gauge section and, if possible, between the contact points of the extensometers. The contact pressure used to attach the extensometers to the specimen should be large enough to prevent slippage but insufficient to indent the specimen surface. Strain gauges are not recommended as they locally stiffen the specimen [1]. Values for Young's modulus and Poisson's ratio are calculated from the regression slopes in the linear region of the T-T and t-T curves. Use of regression slopes is preferable to single point values owing to the potential scatter in the data points (particularly the t-T data) that is mainly due to uncertainties in the small extensions measured. Whilst elastic values can be determined over any strain range where the data appear linear, the slight curvature due to viscoelastic effects will tend to reduce the value of E as the strain range widens. The measurement of tensile hardening curves involves use of the same tests out to larger strains. Contacting extensometers, unless they have been modified, typically have an upper strain limit of around 0.05. They may also initiate premature failure in the specimen at a point of contact. For these tests, the use of a video extensometer is therefore preferable for the measurement of axial strain. The videoextensometer gauge markings are visible on the tensile test specimen shown above. These instruments are generally unsatisfactory for the measurement of small displacements and so a contacting device is best used to measure the lateral strain for the determination of true stresses and the plastic component of Poisson's ratio. 1. G.D. Dean and B.C. Duncan, Preparation and Testing of Bulk Specimens of Adhesives. NPL Measurement Good Practice Guide No 17, July 1998. 2. ISO 3167:1993, Plastics - Multipurpose test specimens. 3. ISO 527-2:1993, Plastics - Determination of tensile properties - Part 2: Test conditions for moulding and extrusion plastics. BACK HOME

Tensile DataNominal Strain 0.0004 0.0015 0.0035 0.0053 0.0070 0.0086 0.0103 0.0120 0.0135 0.0153 0.0172 0.0189 0.0211 0.0230 0.0251 0.0274 0.0298 0.0322 0.0348 0.0373 0.0399 0.0423 0.0452 0.0476 0.0504 0.0533 0.0560 0.0588 0.0615 0.0643 0.0670 0.0699 0.0728 0.0758 0.0786 0.0812 0.0842 Nominal Stress (MPa) 1.44 4.80 10.34 15.73 20.71 24.28 28.02 31.59 34.93 37.89 40.46 43.13 45.03 46.81 48.57 49.68 50.65 51.46 52.25 52.90 53.36 53.63 54.07 54.46 54.80 54.98 55.33 55.84 55.97 56.19 56.32 56.44 56.79 56.86 57.09 57.17 57.26

Here are typical tensile data for a rubber-toughened epoxy. The data are shown in tabular and graphical form.

BACK

HOME

Tensile Data for Elastic-Plastic ModelsElastic-plastic models in FE systems require data in the form of elastic constants to describe elastic behaviour and parameters that describe the yield, hardening and flow behaviour to describe plastic (non-linear) behaviour. Further information on elastic and plastic behaviour is available. Data from t

*View more*